Presentation on theme: "ERC/NSM and CPF- The Ohio State University"— Presentation transcript:
1ERC/NSM and CPF- The Ohio State University Application of Viscous Pressure Bulge (VPB) Test to Predict the Flow Stress of Sheet Materials under Biaxial Deformation ConditionsERC/NSM and CPF- The Ohio State UniversityJanuary 20114
2Outline Introduction Principles of Viscous Pressure Bulge (VPB) Test Methodology to Estimate Material PropertiesObjectivesProcedureResultsEvaluation of Formability using the VPB testConclusionsAcknowledgementAvailable Flow Stress dataReferences
3IntroductionAHSS and Al alloys are used increasingly in forming automotive structural parts because of safety and lightweight vehicle requirements.Some of these alloys have higher strength and low formability compare to conventional draw quality steels.One of the problems is the property variations in incoming materials which may not be determined by the tensile test.Tensile test is uniaxial and flow stress data is obtained to small strains, while the bulge test is biaxial and data is obtained to higher strains.
4Principles of Viscous Pressure Bulge (VPB) Test Viscous Pressure Bulge (VPB) test tooling
5Material properties of HSS/AHSS/UHSS Schematic of viscous pressure bulge test setup at CPF (OSU) and EWIClamping forceDie diameter = 4 inches (~ 100 mm)Die corner radius = 0.25 inch (~ 6 mm)Bulge/ Dome height (h)Pressurized mediumInitial StageTesting stagePressure (P)Methodology to estimate material properties from VPB test, developed at CPF (OSU)MeasurementMaterial propertiesFEM based inverse techniquePressure (P)Dome height (h)Flow stressAnisotropy
6Material Properties Determination of Flow Stress Tensile Test 0.15 Ref: Nasser et al 2010
7Results-Tensile TestUniform and Total Elongation of various AHSS grades (Gauge Length: 2 in)
8UTS and 0.2% Offset Yield Strength of various AHSS grades Results-Tensile TestUTS and 0.2% Offset Yield Strength of various AHSS grades
9Material properties of HSS/AHSS/UHSS Bulge test samplesBefore burstingAfter bursting9
10Material Properties Determination of Flow Stress Bulge Test 0.49 Challenges:Tensile test gives a very limited information,Bulge test gives more reliable strain-stress data.10Ref: Nasser et al 2010
11Materials Tested with VPB Test at CPF and EWI Steels and Stainless SteelsSt 14DP 780-CRSt 1403DP 780-HYAISI 1018Bare DP 980 Y-type XAKDQBare DP 780 T-Si type1050GA DP 780 T- AI TypeDR 120GA DP 780 Y-type UDDSGA DP 780 Y-type VBH 210 DQS-270F GA-Phosphate coatedHSS DQS-270D GA-Phosphate coatedDP500SS 201DP 590SS 301DP 600SS 304DP 780SS 409TRIP 780AMS 5504DP 980Aluminum and Magnesium AlloysAA 6111AA 5754-OAA 5182-OX626 -T4PAZ31BAZ31B-OMaterials Tested at EWI-FCAA-X620270EDP 980TRIP 980TWIP 980TRIP 1180
12Evaluation of Formability Graph shows dome height comparison for SS409 sheet material from eight different batches/coils [10 samples per batch]Highest formability G , Most consistent FLowest formability and inconsistent H
13ConclusionsStrain values obtained in the VPB test is higher than values obtained in the tensile test. Thus, VPB test is more suitable for providing flow stress input to Finite Element Analysis (FEA).Some materials may behave differently under different states of state. VPB is closer to actual stamping operations than the uniaxial tensile testFor some materials, correcting the flow stress obtained from the VPB test for anisotropy may be important.Dome Height at bursting in the VPB test is a quick and reliable test to check the quality of incoming raw materials (different batches, suppliers, …) under biaxial state of stress.Large amount of data may be lost (AHSS) when ending the VPB before bursting. Thus, it is desirable to end the test as close, to the burst pressure , as possible.